Three new solvent-directed 3D lead(II)-MOFs displaying the unique properties of luminescence and selective CO2 sorption.
Li, Jiang; Yang, Guoping; Hou, Lei; Cui, Lin; Li, Yuanpu; Wang, Yao-Yu; Shi, Qi-Zhen; Dalton transactions (Cambridge, England : 2003) 42 (2013) 13590–13598; doi:10.1039/c3dt51203g

data_7023342
_publ_section_title
;
 Three new solvent-directed 3D lead(II)-MOFs displaying the unique
 properties of luminescence and selective CO2 sorption.
;
_journal_issue                   37
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13590
_journal_page_last               13598
_journal_paper_doi               10.1039/c3dt51203g
_journal_volume                  42
_journal_year                    2013
_chemical_formula_sum            'C30 H14 N9 O12 Pb3'
_chemical_formula_weight         1314.07
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 116.3860(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   15.3197(14)
_cell_length_b                   15.6843(15)
_cell_length_c                   15.1838(14)
_cell_measurement_reflns_used    2349
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      21.7145
_cell_measurement_theta_min      2.5975
_cell_volume                     3268.3(5)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0559
_diffrn_reflns_av_sigmaI/netI    0.0685
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            16284
_diffrn_reflns_theta_full        25.10
_diffrn_reflns_theta_max         25.10
_diffrn_reflns_theta_min         1.48
_exptl_absorpt_coefficient_mu    15.497
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.91404
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   sadabs
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    2.671
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2396
_exptl_crystal_size_max          0.30
_exptl_crystal_size_mid          0.24
_exptl_crystal_size_min          0.21
_refine_diff_density_max         1.663
_refine_diff_density_min         -1.598
_refine_diff_density_rms         0.461
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.934
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     489
_refine_ls_number_reflns         5811
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.934
_refine_ls_R_factor_all          0.0642
_refine_ls_R_factor_gt           0.0392
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0890P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1033
_refine_ls_wR_factor_ref         0.1368
_reflns_number_gt                4336
_reflns_number_total             5811
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c3dt51203g.txt
_cod_data_source_block           2
_cod_original_sg_symbol_H-M      P2(1)/c
_cod_database_code               7023342